Phonon frequency spectrum through lattice dynamics and normal coordinate analysis of htsc tl2 ca3ba2cu4o12
1.
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol 5, 2012 Phonon Frequency Spectrum through Lattice Dynamics and Normal Coordinate Analysis of HTSC Tl2Ca3Ba2Cu4O12 K.Sonamuthu* J.N.R.Mahavidyalaya, Port Blair, Andaman India) *E-mail:sona_muthu2008@rediffmail.com(Contact Cell; 09474223678)AbstractThe lattice dynamics of the high temperature superconductors Tl2Ca3Ba2Cu4O12 has been investigated on thebasis of the three body force shell model (TSM). The various interactions between ions are treated on a generalway without making them numerically equal. The phonon frequency at the zone centre of Brillouin zone arepresented and the vibrational assignments are discussed. Further the normal coordinate calculation has alsobeen employed to study the vibrational analysis of this compound. The normal coordinate analysis of thesuperconductor Brillouin zone has been calculated by using Wilson’s F-G matrix method which is useful forthe confirmation of our present investigation. The vibrational frequencies and the potential energy distribution(PED) of the optically active phonon modes are also presented.Keywords: Lattice dynamics, Normal Coordinate, Brillouin zone, Three shell Force shell Model,Tl2Ca3Ba2Cu4O12, Zero Wave Vector, high-temperature superconductors, Raman, infrared. PhononFrequency ,etc.1. IntroductionThe study of the lattice dynamics of the high-temperature superconductors is of importance not only for theoverall physical characterization of these compounds but also for an assessment of the role played by thephonons i.e., the superconducting phenomenon. A lattice dynamical study requires the knowledge of the crystalstructure and the particle interactions. Usually the crystal structure is determined using X-ray diffraction. Forparticle interactions one has to use models, which represent the characteristic of the electronic structure and itseffect on ionic interaction in a relevant manner. In lattice dynamics the ionic interactions are expressed intermsof force constants. Cox et.al. (1988) have refined the structure of high-temperature superconductorsTl2Ca3Ba2Cu4O12 using neutron and powder diffraction data. Raman and infrared active modes ofTl2Ca3Ba2Cu4O12 have been calculated by Kulkarni et al.(1989) in the frame work of shell models.Belosiudov et al. (1991) have calculated vibrational spectrum of Tl2Ca3Ba2Cu4O12 using interatomic interactions.A high resolution neutron diffraction study on Tl2Ca3Ba2Cu4O12is contributed by Ogborne et.al (1992).In the present work we start with a more general approach in the framework of the three body-force shell model(TSM) with R # S # T to calculate the lattice dynamics frequencies. The values of the phonon frequenciescalculated in this present work at zone center by the three body force shell model is in good agreement with theavailable Raman and infrared values. Further a normal coordinate analysis has also been attempted for thesuperconductor Tl2Ca3Ba2Cu4O12 using Wilson’s F-G matrix method for the confirmation of our presentinvestigations. The vibrational frequencies and the potential energy distribution (PED) of the optically activemodes are also reported.2. Theoretical Consideration2.1 Lattice dynamics of Tl2Ca3Ba2Cu4O12based on the shell modelThe calculation of lattice dynamical vibration frequencies of Tl2Ca3Ba2Cu4O12system is performed by three-bodyforce shell model (TSM) calculations. In the shell model calculation the equations of the motion for the codecoordinate U and the shell coordinate W are expressed as follows: -Mϖ2U= (R + ZCZ) U + (T + ZCY) W 0 = (T – YCZ) U (S + K + YCY) W （1）With ZCZ = Z[Z + 2f (a)] C + V where M, Z and Y are diagonal matrices representing the mass ionic charge onthe shell. R, S and T are matrices specifying short–range core-core, shell-shell and core-shell interactions,respectively. V is the matrix describing the three-body overlap interactions andf(a) is related to overlap integrals of electron wave function. U and W are the vectors describing the ionicdisplacements and deformations respectively. 15
2.
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol 5, 2012In the earlier approaches the R, S and T elements were considered to be equal to one another. In the presentinvestigation, we have started with an approach such that R # S # T (Moha., et al. 1986). That is the variousinteractions between the ions are treated in a more general way without making them numerically equal. Thedynamical matrix of the model consists of long-range Coulomb and three-body interactions and the short-rangeoverlap repulsions. The off-diagonal elements of this matrix along the symmetry directions chain a completelynew term having a significant contribution for unequal R, S and T.The lattice dynamical calculation of high-temperature superconductors is explained using an interionic potentialconsisting of long-range Coulomb part and a short-range Potential of Born-Mayer from (Onari,S., et al. 1988) Vij = aij exp (-bij r) （2）Where i, j label the ions and r is their separation. The parameters aij and bij are the pair potentials and theparameters Y and K determine the electronic polarizabilities. The parameters used in the present calculations aregiven in Table 1. Phonon frequencies are calculated using the force constants derived from the interionicpotential. Following (Leaner et a1. 1982) interionic pair potentials for short-rang interactions can be transferredfrom one structure to another in similar environments. The force constants evaluated by this method are in goodagreement with the evaluated values ( Onari,S., et al 1990; Thomsen, C., et al.1987).2.2 Normal Coordinate Analysis of the Zero Wave Vector Vibrations of Tl2Ca3Ba2Cu4O12The high Tc superconductor Tl2Ca3Ba2Cu4O12 System crystallizes in the simple tetragonal (st) system, whichbelongs to the space group P4/mmm(D′4h) The simple tetragonal (st) unit cell of Tl2Ca3Ba2Cu4O12 and thenumbering of the atoms are shown in Fig.1. The 21 atoms of the unit cell yield a total of 42 optical vibrationalmodes. All the above calculations are made at q = 0. Once of A2u and Eu modes corresponds to acousticvibrations with frequency ω = 0. These normal modes are distributed as follows.A2u + Eu from the motion of a Tl atomsAlg + Eg + A2u +Eu from the motion of 2 Ca atomsA2u + Eu from the motion of a Ca atomsAlg + Eg + A2u + Eu from the motion of 2 Ba atoms2Alg + 2Eg + 2A2u + 2Eu from the motion of 4 Cu atoms2A1g + 2B1g + 2Eg +2 A2u +2 B2u + 3Eu from the motion of six O (1) atoms along c-axis.A1g +2 Eg + A2u + B2u + 2Eu from the motion of four O(2) atoms along b-axisEg + A2u + B2u + Eu from the motion O (4) atoms along a-axisSubtracting the translation modes A2u + B2u + Eu the q = 0 optical modes involved in an irreduciblerepresentation are as follows. Γopt = 7A1g + 2B1g + 9Eg +10A2u + 2B2u + 12Eu （3）The species belonging to A1g and Eg Raman active modes whereas A2u Bu are infrared active modes. The A2uand A1g modes involve displacement along crystallographic c-axis, the B2u and Eg modes along the b-axis and Eumodes along the a-axis. The normal coordinate calculation was performed using the programs GMAT andFPERT given by (Fuhrer et al.1976). The general agreement between the evaluated and observed normalfrequencies of Tl2Ca3Ba2Cu4O12 is good. The calculated force constants using the above programs are given inTable 2. It is interesting to note that the evaluated frequencies given in Table 3. agree favourably with theexperiment values.The normal coordinate calculation was performed using the programs GMAT and FPERT given (Fuhrer etal.1976). The general agreement between the evaluated and observed normal frequencies of Tl2Ca3Ba2Cu4O12 isgood. The calculated force constants using the above programs are given in Table 2. It is interesting to note thatthe evaluated frequencies given in Table 3 agree favourably with the experimental values.To check whether the chosen set of vibrational frequencies makes the maximum contribution to the potentialenergy associated with the normal coordinate frequencies of the superconducting material, the potential energydistribution was calculated using the equation. 16
3.
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol 5, 2012 PED = (F ij L 2 ik) / λk (4)Where Potential Energy Distribution (PED) is the combination of the i-th symmetry coordinate to the potentialenergy of the vibration whose frequency is ν k, Fij are potential constants, Lik, are L matrix elements and λk = 4π2 C2 ν2k. 3. Results and Discussion:3.1 Lattice Dynamical Calculation using Shell Model(Tl2Ca3Ba2Cu4O12) The Lattice Dynamical calculations based on modified TSM reproduce the observed frequencies of Raman andinfrared active modes reasonable which are given in table 3. The calculated frequencies are in good agreementwith the available experimental values. The lowest calculated Raman active A1g mode frequency at 101cm-1 isdue to the vibration of Ba atoms and this agrees very well with the experimental frequency at104cm-1. Similarly the calculated Raman frequency in A1g symmetry at 126 cm-1 and 449 cm-1 are due to thevibration of Tl and O(1) atoms respectively and the observed frequencies at 127 and 459 cm-1 agrees very wellwith the calculated frequency. The highest calculated Raman frequency 528 cm-1 in A1g symmetry is due to thevibration of O(2) atoms which also agrees very well with the observed frequency at 528 cm-1.The Raman Phonon frequency at 206 and 298cm-1 in B1g symmetry are due to the vibration of O(1) and O(4)atoms respectively.The calculated Raman Phonon frequency in Eg symmetry at 68 cm-1 244cm -1, 399cm -1, 545cm -1 are due to thevibration of Ba1, Cu1 , O(2) and O(3) atoms respectively and it agrees very well with the observed frequencies at65 cm -1, 245cm -1, 400cm -1 and 545cm -1 respectively.The phonon frequencies at 107cm -1 is due to the vibration of Ba, Ca and Cu. The Ca and Cu vibrates at 180 0out of phase to Ba atom. Similarly the calculated phonon frequency at 365cm -1 is due to the vibration of O(4)atom , which is out of phase to O(1) atom and its observed frequency at 365cm -1 agrees very well with thecalculated phonon frequencies. The calculated Raman phonon frequency at 398 cm -1 is due the vibration due tothe O(1) atom and it performs bending bond vibration in the O(4) atom and Ca atom is out of phase to O(1) andO(4) atom. The observed frequencies at 398 cm -1 agrees very well with the calculated phonon frequencies. Thehighest phonon frequencies in symmetry Eg is due to the vibration of O(4) atom and performing stretching bondvibration.The Calculated IR frequency in A2u symmetry at 79cm-1 and 143cm-1 are due to the vibrations of Cu(1) andCu(2). The frequencies at 139cm-1 is due to the vibration of Tl and Ba atom. The frequency at167cm-1 is due to the vibration of Ca, O(1) and O(4) atoms and its observed frequency at 157cm-1 is agrees verywell with calculated frequencies. Similarly the frequency at 295cm-1 is due to vibration of O(1) and O(2) and Caatoms and Ca atom vibrates at 1800 out of phase to O(1) and O(2) atoms. Its observed frequency at 313cm-1agrees very well with the calculated phonon frequency. Therefore the calculated infrared frequency 456 cm -1 isdue to the vibration of Ca, O(1) and O(2) atom where as O(1) atom vibrates at 1800 out of phase to Cu and O(2).The highest frequency in A2u symmetry is 570cm-1 is due to vibration of O(3) atom and its observed frequencyis 574cm-1 agrees very well with the calculated frequency.The calculated Infrared frequency in B2u symmetry at 126cm-1 and 284cm-1 are due to vibration of O(1) andO(4) atoms respectively.The calculated infrared frequencies in Eu symmetry at 68cm-1 is due to vibration of Tl atom and its observedfrequency 68cm-1 agrees very well with the calculated frequency. The calculated frequency at 247cm-1,375cm-1, 380cm-1 are due to the bending bond vibration and it agrees with observed frequencies at 247cm-1,372cm-1 and 380 cm -1 agrees very well with the calculated frequencies. To calculate frequencies at 559cm-1and 568cm-1 are due to vibration of O(1) and O(4) atoms respectively performing stretching bond vibration andits observed frequency 559 cm-1 and 568cm-1 agrees very well with the calculated phonon frequency. Theobserved frequencies at 565cm-1 agrees very well with the phonon frequency.3.2 Normal co-ordinate analysis of Tl2Ca3Ba2Cu4O12The evaluated frequencies using the normal coordinate analysis method listed in table 3. agrees favourably withthe calculated lattice dynamical frequencies and observed experimental frequencies.The calculated Raman phonon frequency in A1g symmetry at 107cm-1 is due to the vibration of Ba atomwhich is the lowest frequency in this mode due to the stretched vibration of Ba-O(2). The calculated frequency at124cm-1 is due to the vibration of Tl atom which is due to the stretched vibration of Cu-O(1). The frequencyat 147cm-1 is due to the vibration of O(1)-Cu-O(1). Similarly the highest frequency in this symmetry 530cm-1 isdue to the vibrations of O(2) atom and it is due to the bending vibration of O(1)-Ca-O(2) which agrees very well 17
4.
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol 5, 2012with the observed frequency at 528cm-1, which is confirmed potential energy distribution calculation.The frequency at 60cm-1 in Eg symmertry is due the vibration of Ba atom which is due to stretched vibration ofBa-O(2). The calculated frequency at 390 cm-1 is due to the vibration of O(1) atom and it is due to bendingvibration of Tl-O(2)-Ba. The highest frequency in this symmetry is 560cm-1 is due to the vibration O(4) atomwhich is due to the stretched vibration. This frequency agrees very well with the observed frequency at 567cm-1which is confirmed by potential energy distribution calculation.The lowest frequency in the A2u symmetry is 80cm-1 is due to the vibration of Cu(1) atom which is due to thebending vibration Tl-O(3)-Tl. The calculated frequency at 300cm-1 is due to the vibration of O(2) atom which isdue to the bending vibration O(1)-Cu-O(1). The highest calculated frequency in this symmetry is 588 cm-1,which is due to the vibration of O(3) atom which performs stretched vibration of Ca-O(1). The calculatedfrequency agrees very well with the calculated frequencies is confirmed by potential energy distributioncalculation.The calculated frequency in Eu symmetry at 70 cm-1 is due to the vibration of Cu(2) atom and which is due tobending vibration of O(2)-Tl-O(3). The frequency at 365 cm-1 is due to the vibration of O(1) atom and whichis due to the bending vibration. The highest calculated Infrared Raman frequency 570 cm-1 is due to thevibration of O(4) atom which is performed by stretched vibration of Tl-O(4).The G-matrix elements have been calculated from the equilibrium geometry. The initial force constants weretaken from the related molecules. The final set of potential constants provide the stability of the crystal inrelation to all vibrational modes. The vibrational frequencies and potential energy distribution values arepresented in this work. The potential energy distribution indicates the contribution of an individual forceconstant to the vibrational energy of normal modes. It clearly indicates that there is mixing of the internaldisplacement coordinates.Vibrational modes on the region 400-500 cm-1 are attributed to Ca-O(2) stretching. The present potentialenergy distribution confirms our conclusion. The lower frequency modes involve the small displacement ofCa-O(2) and Ba-O and the angular displacement of O-Ca-O. The evaluated frequencies using the normalcoordinate analysis method listed in table 3 agree favourably with the calculated lattice dynamical frequenciesand observed experimental frequencies.4.Conclusion The theoretical phonon frequencies obtained by the lattice dynamics and the normal coordinate analysis methodagrees very well will the available Raman and infrared frequencies. This calculation attributes not only thephonon frequency in center of the Brilioun zone but also supports the strong electron-phonon interaction in thehigh-temperature superconductor Tl2Ca3Ba2Cu4O12.methods viz, lattice dynamical study and normal coordinate analysis yielded the same phonon frequency forTl2Ca3Ba2Cu4O12 high temperature superconductor. It is also seen from the tables, that the agreementbetween the calculated and observed frequencies wherever available are very good for the system underconsideration. This fact supports It is not uncommon in physics that two different methods yield the same result.In the present work, two different that the present vibrational assignments made for the infrared and RamanSpectra are adequate. Therefore, it is concluded that normal coordinate analysis of the optically active latticevibrations is very useful for the theoretical interpretation of the vibrational spectra at the center of the Brillouinzone in cuprate oxides. Further it is also a good method to characterize the high temperature superconductors.It is also shown that it is possible to obtain is a fairly reasonable representation of the lattice vibration inTl2Ca3Ba2Cu4O12. Using the three-body force shell model, with the assumption of unequal short-rangeinteractions, the present approach leads to yields a complete phonon frequency of high Tc superconductor underconsideration in the present work. Summarizing, the theoretical phonon frequencies obtained by the latticedynamics and the normal co-ordinate analysis agree very well with the available Raman and infraredfrequencies.AcknowledgementThe author is thankful to referee whose critical comments were of great help in improving the paper to thepresent form. The author is also grateful to Prof S.Mohan, Vice Chancellor of Prist University, Tanjavur, TamilNadu,India for providing facilities to carry out this work. 18
5.
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol 5, 2012Reference[1] Cox, D.E., Tovovaradi , C.C., Subramanian, M.A., Gopalkrishnan, J., and Sleight, A.W. , (1988), Phys. Rev. B 38, 6624.[2] Kulkarani , A.D.,. Pride, J., DE Watte, F.W. , KRESS, W., and Schroder. U., (1989), Phys. Rev. B 40, 2624.[3] Belosludov , V.R. , Lavrentiev, M.Y. , and Syskin, S.A., Int. J.Mod. (1991),Phys. B 5, 3109[4] Ogborne , D.M. , Waller, M.T. , and Lanchester , P.C., (1992) Physica C 200, 207[5] Mohan, S., Durai, S., and Vaityanathan. G. ,(1986), Indian J.Phys. 60A, 137[6] Onari , S. ,. Hiroaki, T. , Onghime, K., Honme, H., and Arai, T., (1988), Solid State Commun. 3. 303[7] Lehner , N., Rauh, H., Strobel, K., Geick, R., Heger, G., Bouillot, J., Renker, B., Rousseau. M., and Stirling. W.J. , (1982), J. Phys. C 15, 6545.[8] Onari, S., Ono, A., Arai,T., and MORI , T., (1990), Physica B 165/166, 1235.[9] Thomson , C., Cardona, M., Kress, W., Genzel, L., Bauer, M., King, W., and Wittlin, A., (1987), Soild State Commun. 64, 727[10] Fuhrer , H., Kartha, V.B. , Kidd, K.G., Krueger, P.J. , and Mantasch, H.H. , (1976),Computer Programs for Infrared Spectrometry, Vol. V, Normal Coordinate Analysis National Research Council of Canada, Ottawa.AuthuorThe author is born (DOB-03/06/1966) and brought up at Port Blair, Andaman, India. The author has completedM.Sc in Physics in the year 1993 from the American College Madurai, Tamil Nadu. I have completed my Ph.Din High Temperature Superconductors in the year 2003 from Pondicherry University Pondicherry, India. Atpresent I am working as a Associate Professor in Physics at JNRM., Port Blair, Andaman and Nicobar Islands,India. Fig. 1 Unit Cell of Tl2Ca3Ba2Cu4O12 19
6.
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol 5, 2012Table :1Parameters of the model: a, b are Born- Mayer constants: Z, Y, K, ionic charge, shell charge and on-sitecore-shell force constant of the ion, va is the volume of the unit cellInteraction a (eV) b (Å -1)T1-O (Same plane) 3000 2.80T1-O (adj plane) 3000 3.55Ba-O 3220 2.90Ca-O 2510 3.10Cu-O 1260 3.35O-O 1000 3.00______________________________________________________________________ion Z(|e|) Y(|e|) k(e2|va)______________________________________________________________________T1 2.70 2.00 1000Ba 2.00 2.32 207Ca 2.02 -0.50 1350Cu 2.00 3.22 1248O(Cu-O) plane -1.90 -2.70 310O(T1-O) plane -1.93 -2.70 210O(Ba-O) plane -1.93 -2.70 310 (K||) 2100(K┴)______________________________________________________________________ 20
7.
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol 5, 2012Table : 2Force constants for Tl2Ca3Ba2Cu4O12 (in units of 102 Nm-1 (stretching) and 10-18 Nmrad-2 (bending))______________________________________________________________________Potential bond type distance (Å) initial valueConstantsfa Ca-O(1) 2.467 1.06fb Ba-O(1) 2.798 0.75fc Ba-O(2) 2.819 1.10fd Ba-O(3) 2.851 0.81fe Tl-O(1) 2.003 0.30fg Tl-O(2) 2.097 0.30fh Tl-O(3) 3.108 0.61fk Tl-O(3) 2.402 0.48fl Cu-O(1) 1.932 0.145fm Cu-O(2) 2.648 1.65fn Tl-O(3) –Tl --- - 0.31fp O(1)-Cu-O(1) ---- 0.25fα Tl-O(2)-Ba ---- 0.46fβ O(2)-Tl-O(3) ---- 0.80 21
8.
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol 5, 2012 Table:3. The Phonon frequency Spectrum of Tl2Ca3Ba2Cu4O12. Symmetry Frequency(cm-1) Using Normal PotentialEnergy species Using Lattice Coordinate Distribution(%) Dynamics analysis A1g (Raman) 101 (104) 107 f c (58) f d( 24) fa (11) 126 (127) 124 f c (55) fl (30) 148 (142) 147 fl(71) fd (12) fp(11) 256 (256) 256 fa (51) fα(20) 370 (360) 377 fa (68) fu(20) fc (10) 449 (439) 438 fa (61) fc (20) fm (10) 528 (528) 530 fa (59) fe(29) fm(11) 625(628) 630 Fl (69) fe(19) fm(17) B 1g 206 210 fa (56) fk (14) fa (10) 298 296 fa(52) fk (20) f β (6) Eg 68(65) 60 fc (60) fe (14) f β (6) 107(107) 110 fm (70) fe(18) f β(10) 125 (125) 125 fm (70) fl (21) 244 (245) 240 fe (52) fm (16) fc (12) 3656 (365) 370 fl(45) fn(31) fc(20) 378 (400) 390 fa (42) fg (25) fn(15) 399 (410) 405 f β(56) fk (17) fg(16) 545 (54) 550 fn (62) fh (22) fm(14) 555 (567) 560 fα (68) fn(21) A2u 79 (79) 80 fn (70) fa(24) 139 (137) 136 fm(65) fu(20) fd(11) 143 (143) 150 fm(80) fl(14) 160 (167) 165 fa(81) fe(16) 295(313) 300 fp(54)fn(30) 422 (432) 430 fp(62) f β(18) fn(10) 432 (437) 440 fa(40) fg(30) fn(10) 456 (450) 450 f β(41) fp(21) fm(26) 570 (574) 580 fa(60) fe(21) fm(16) B2u 126 130 fp(54) fn(26) fe(15) 284 283 f β(28) fp(21) fu(30) fe(19) Eu 68(68) 70 f β(70) fc(20) 107 (107) 110 fa(71) fe(20) 132 (133) 134 fa(46) fd(18) fb(10) 247 (247) 247 fn(52) fa(17) fe(24) 255 (255) 250 fa(55) fd(18) fc(10) 355 (36) 365 fc(61) fe(16) fu(14) 375 (372) 378 fa(55) fe(14) fu(20) 380 (380) 381 fp(64) fc(16) 455 (455) 460 f β(66) fp(25) 559 (559) 562 fn(65) fα(21) 568 (568) 570 fn(68) fa(25) 22
9.
This academic article was published by The International Institute for Science,Technology and Education (IISTE). The IISTE is a pioneer in the Open AccessPublishing service based in the U.S. and Europe. The aim of the institute isAccelerating Global Knowledge Sharing.More information about the publisher can be found in the IISTE’s homepage:http://www.iiste.orgThe IISTE is currently hosting more than 30 peer-reviewed academic journals andcollaborating with academic institutions around the world. Prospective authors ofIISTE journals can find the submission instruction on the following page:http://www.iiste.org/Journals/The IISTE editorial team promises to the review and publish all the qualifiedsubmissions in a fast manner. All the journals articles are available online to thereaders all over the world without financial, legal, or technical barriers other thanthose inseparable from gaining access to the internet itself. Printed version of thejournals is also available upon request of readers and authors.IISTE Knowledge Sharing PartnersEBSCO, Index Copernicus, Ulrichs Periodicals Directory, JournalTOCS, PKP OpenArchives Harvester, Bielefeld Academic Search Engine, ElektronischeZeitschriftenbibliothek EZB, Open J-Gate, OCLC WorldCat, Universe DigtialLibrary , NewJour, Google Scholar
Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.
Be the first to comment